A comparison of Properties of laboratory prepared Cold Mixed Emulsified and Hot MixedAsphalt Mixtures
Jack N Dybalski, Manager Asphalt Technology, Akzo Chemicals Inc., McCook Illinois
Presented at the 10th Annual Meeting of the Asphalt Emulsion Manufacturers AssociationMarch 22-25 1983 Palm Springs California
Abridgement of report prepared for Akzo Chemicals Inc. by Western Technologies Inc PhoenixAZ, December 1982
TABLE OF CONTENTS
1.0 Summary . . .
4.0 Specimen Preparation
5.0 Data Matrix
6.0 Tests and Measurements
7.0 Effect of Binder Type
6.0 Effect of Gradation
9.0 Effect of Anti-Strip Treatment
10.0 Effect of Compaction Method
11.0 Effect of Cure Method
12.0 Conclusions and Recommendations
13.0 Addendum : Cure Method Variations
Asphalt emulsion cold mixes for construction of base and surface courses of bituminouspavements have been used in the United States since the 1930~s. These mixes were primarilyused on lightly traveled roads with very little, if any, documentation of their physical propertieseither before or after construction. In addition, until recently very little effort was made todevelop a generally acceptable laboratory design method for asphalt emulsion cold mixes. Amethod which engineers could use as a tool for comparison to other asphalt paving materials andmethods for pavement thickness determinations5
During the past ten years Armak Company has expended a considerable amount ofinvestigative and developmental effort toward determining those factors which are mostimportant in developing an acceptable laboratory design method for asphalt emulsion cold mixesand those factors which are necessary to obtain layer equivalency to hot mix. Concurrently,asphalt emulsion formulations of the cationic type that would adequately mix with almost anytype of aggregate without the benefit of the lubricating effect of solvent, were developed and arestill being refined5 These formulations, which solely rely upon the inherent properties of theemulsifier and the proper use of water, are essential for preparing cold mixes that adequatelycompare to the pavement-thickness criteria of hot mix.
Simply stated, in the field, asphalt emulsion layer equivalency to hot mix can be attainedby: (1) having field paving crews learn the proper use and handling of water and solvent-freecationic asphalt emulsions, (2) the use of an asphalt cement in the cold mix which is similar inviscosity or stiffness to the asphalt cement recovered from the hot mix, and (3) allowing the coldmix to cure to near its optimum stability, keeping all other variables equal.
Developing an acceptable laboratory design method for cold mixes, which reflects theirpotential equivalency to hot mix in the field, has been considerably more difficult.
Armak has, thus far, sponsored two studies at an independent testing laboratory todetermine those factors which most significantly effect the mix design criteria and resilientmoduli of asphalt emulsion cold mix compared to hot mix using two different laboratory ofspecimen preparation and evaluation -- Marshall ASTM, D-1559 and Kneading CompactionASTM, D-1561 with the Hveem Method ASTM, D-1560.
Phase I of this investigation was reported at the AEMA Annual meeting, March 17-18,1982, Las Vegas, Nevada.
The premise of this initial investigation was to emulsify an asphalt cement that hasviscosity (stiffness) properties similar to the asphalt extracted from a hot mix after the hot mixinghad been completed and to use the emulsion in the preparation of cold mixes for comparison tothe original hot mix. This was done to determine whether a cold mix versus a hot mix, bothcontaining asphalt cement of similar stiffness or viscosity, would indicate similar pavementthickness requirements.
The cold mix formula used 2% pre-wet water basis dry weight of aggregate and four setsof three specimens each at 4.0, 4.5, 5.0 and 6.0 residual asphalt respectively. A CSS-1. asphaltemulsion which contained no volatile hydrocarbon was used for the cold mix. The.hot mixspecimens were also prepared at the same asphalt content for direct comparison.
The Marshall Method of lab specimen compaction and testing was used to obtain specimendensity and stabilities. With the development of the densitylair voids data, it became evident thatMarshall Compaction, as detailed in ASTM D-1559, is not the best tab method of compaction forthese cold mix specimens. Densities and air voids equivalent to that of the hot mix wasimpossible to obtain with the Marshall Compaction Hammer, particularly with the denseaggregate.
The major problem with specimen compaction for cold mixes using the Marshall Methodis that it was designed for hot mix which contains only trace volatiles at compactiontemperatures. The mold assembly is non-porous and the tamping foot of the compaction hammeris essentially the same diameter as the inside diameter of the mold. Although 50 to 75 blows ofthe Compaction Hammer are specified for each flat side of the specimen, the water containingcold mixes often attain maxi(num attainable density after only 20 blows with rapidly developinghydraulic pore pressure causing the hammer to bounce for the remaining blows and generatingan accumulation of emulsified asphalt on the flat surfaces of the specimen.
Some work has been done with the Marshall Compaction of specimens in porous molds.However this approach has not been found to be entirely adequate because of insuffieientreduction of pore pressure under the tamping foot of the Marshall Hammer and the tendency ofsome aggregate projections to become wedged in the holes causing specimen tearing whenremoved from the mold.
Suprisingly the Resilient Modulus (Mr) (elastic Modulus) data is considerably higher for theemulsion mixes than for the hot mixes. Resilient Modulus (ElasticModuli) values have manymeanings to design engineers; however, if only these numbers were used to determine pavementthickness design, they would imply that the hot mix should be placed thicker than the cold mixfor equivalent load bearing.
This study - Phase II - used the same aggregates, Arizona Types IIIb and IVb, and thesame asphalts and AR-8000 for the cold mix and an AR-4000 for the hot mix which, whenextracted from the hot mix, has essentially the same penetration and viscosity (stiffness) as theAR-8000. Phase II, however, investigated the compaction characteristics of KneadingCompaction and the Hveem stability procedure in contrast to the Marshall method reported inPhase I. Phase II also reports the results of accelerated laboratory specimen cure in an effort toobtain density and voids values similar to the high density and low voids obtainable from coldmix placed in the field.
Kneading compaction appears to produce specimens of higher density and lower voidsthan does the Marshall. However, both methods are inadequate, as written, to obtain the densityand voids values which are comparable to the high density and low voids which are possiblefrom a 3" to 4" mat of cold mix placed in the field.
These data indicate that an appropriate laboratory specimen cure method is more importantthan the method of compaction. This will be the subject of Phase I[I.
The most important need the asphalt emulsion industry currently faces, with respect to coldmix base and surface courses, is the need for well documented and thoroughly tested fieldinstallations where data on density, voids and the development of specification stability withtime can be acquired and disseminated. These data and only these data will validate thedevelopment of a laboratory design method and acceptable design criteria.
This is a summary of a study conducted for Armak by Western Technologies, ~nc. ofPhoenix, Arizona that is a continuation of previous work that showed cold mixed pavingmixtures can be substituted on a 1 to 1 thickness basis for conventional hot mixed asphaltconcrete.
This work is intended to show the effects of aggregate gradation, compaction method,curing method, and anti-strip treatments on laboratory properties of mixtures usi~g emulsifiedasphalt and asphalt cement binders. Properties measured include:
2.1 Aggregates were crushed river gravel from Salt River siliceous deposits in Phoenix,Arizona. Gradations were dense and open conforming to The Asphalt Institute Types IV-b andIll-b as shown on Figure 1.
2.2 Asphalt cement binder was a California AR-4000. emulsified asphalt binders wereformulated solvent-free from a California AR-8000 base stock to approach CSS-1 and CMS-2properties. Anti-strip agent, when used, was Armak Redicote 82-S.
2.3 Binder contents were 4.7 and 4.9 percent by weight of mixture for open and densegradations
3.1 Asphalt cement mixtures were compacted at 230F (110C) by kneading compactor(25 tamps at 250 psi followed by 150 tamps at 500 psi).
3.2 emulsified asphalt mixtures were aerated to optimum compaction fluids content thenreceived 25 tamps of a kneading compactor at 250 psi followed by static doubleplunger loading to 40,000 pounds (177.9 kN). Following compaction, specimenswere cured in the mold for 18 hours at room temperature. After removal from molds,specimens were subjected to 12-15 in Hg (40.5 - 50.6 kPa) vacuum dessication toconstant weight. Other curing methods will be discussed later in this report.
4.0 Data matrix
4.1 Variables considered in the study are shown on Figure 2. Data were analyzed byconventional analysis of variance.
5.0 Tests and Measurements
5.1 The following tests were made as part of the larger study but not all will bediscussed at this time.
Resilient modulus after 18 hour cure
Resilient modulus after full cure
Indirect tensile strength
Eff ec~s of Califcrnia Moisture Vapor Susceptibility conditioning (NvS)
6.0 Effect of Binder Type6.1 Data matrix for this experiment is shown on Figure 3. All mixtures for this
experiment used type Ill-b (open) aggregate gradation. Binders include:
CSS-1: Emulsified asphalt
CSS-1M: Emulsified asphalt modified with an anti-strip additive
CMS-2: Emulsified as~halt
AR-4000: Asphalt cement
AR-4000M: Asphalt cement modified with an anti-strip additive
6.2 Density6.2.1 Cell means are plotted on Figure 4. Hot mixes show statistically higher
densities than cold mixes using emulsified asphalt binders. This is consistent with findings ofpast work and suggests higher voids may be a result of water that remains in the mixture dur~.~;compaction.
6.2.2 Since many mixture design criteria and other laboratory mixturecharacteristics that predict field performance are highly sensitive to density, two questions withregard to mixtures using emulsified asphalt binders must be addressed. The first concernsmoisture removal during field mixing and placement and the second concerns development oflaboratory compaction methods that will accurately simulate field mixtures. Projects are plannedto study both situations and will be reported when results are available and analyzed.
6.3 Resilient Modulus6.3.1 Resilient modulus for hot mixes using asphalt cement averaged 648,000
psi (4.5 GPa) with no significant effects due to the anti-strip modifier. After 18 hours cure,mixtures using emulsified asphalt averaged 117,000 psi (0.8 GPa) with no significant differencedue to emulsified asphalt type or anti-strip modifier. However, after full cure, mixtures usingemulsified asphalt averaged 745,000 psi (5.1 GPa) which is significantly higher than mixturesusing asphalt cement. (See Table 1 and Figure 5)
6.4 Tensile Strength6.4.1 Cell means are plotted on Figure 6. Conventional AR-4000 mixtures
showed a significantly higher tensile strength than mixtures using CMS-2 emulsified asphalt butthere is no statistical difference between mixtures using asphalt cement and CSS-1 emulsifiedasphalt.
6.5 Hveem Stability6.5.1 Stability measurements were made before and after exposure to the
California Moisture Vapor Susceptibility (MVS) test (Caltrans Method 307). The method,essentially, exposes a specimen to 100 percent relative humidity for 75 hours at 140F (60C) priorto stability testing. Caltrans stability requirements are as follows:
Asphalt AsphaltConcrete BaseA B C A B
Stability (mm) 37 35 30 37 35MVS 30 25 20 30 25
6.5.2 As should be expected from density data, stability varies with density.Data for treated and untreated binders are shown on Figure 7. Note that none of the untreatedmixtures meet the criteria for Class A asphalt concrete or base. Both AR-4000 mixtures qualifyfor Class B and the CSS-1 mixture qualifies for Class C.
6.5.3 An interesting observation can be made, however, if percent retainedstability is calculated based on measurement of stability before and after MVS exposure.Ranked averages are as follows:
Binder % Retained Stability
AR-4000M 102.3CSS-1M 102.2AR-4000 91.6CSS-1 81.4CMS-2 80.0
There is statistical significance between binders at the 95 percent confidence level but not at the99 percent level. Mixtures using modified binders show higher retained stability than untreatedbinders and there is no significant difference in retained stability between mixtures using AR-4000, AR-4000M, or CSS-1M. It is of further interest to note that, for all binders, retainedMarshall stability is higher after MVS exposure than dry (before exposure) testing.
7.0 Effect of Gradation
7.1 Data matrix for this experiment is shown on Figure 8. The experiment used bothgradations and CSS-1 and CSS-1M (modified with an anti-strip additive)
7.2 Density7.2.1 There was no statistical effect due to binder type but, as should be
expected, the dense mixtures show higher densities by approximately one lb. per cu. ft.
7.3 Resilient Modulus7.3.1 After 18 hours cure, the CSS-1 type III mixture showed the lowest
resilient modulus (94,000 psi (0.6 GPa)) with no significant differencebetween the remaining three (127,000 psi (0.9 GPa)). After full cure,statistical ranking is as follows:
Mixture Resilient modulus (106 psi)
CSS-1M (IV) 1.32CSS-1 (IV) 1.00CSS-1M (III) 0.78CSS-1 (III) 0.76
7.4 Tensile Strength7.4.1 There is no significant effect due to binder modification but type
IV gradations show higher tensile strengths than type III (147.8 psi (1.0 MPa) vs 108.0 (0.7 MPa)).
7.5 Hveem Stability7.5.1 When analyzed on a percent retained stability basis after MVS there is no
statistical effect due to gradation or binder modification.
8.0 Effect of Antistrip Treatment
8.1 Data matrix for the experiment is shown on Figure 9. This experiment used typeIII gradation and both treated and untreated AR-4000 and CSS-1 binders.
8.2 Hveem Stability8.2.1 When analyzed on a percent retained stability basis after MVS there is no
statistical effect due to base asphalt or anti-strip treatment.
9.0 Effect of Compaction Method
9.1 This section is somewhat subjective in as much as data obtained in this study (25tamps with a kneading compactor at 250 psi followed by a 140,000 pound (177.9 kN) staticdouble plunger load) are compared with 75 blow Marshall data from a different study based onmaterials from the same sources. Data matrix is shown on Figure 10.
9.2 Density9.2.1 There is no statistical effect due to gradation type. Density by the
modified Hveem method was significantly higher than that produced by the Marshall method(143.0 pcf vs 139.7).
9.3 Resilient Modulus9.3.1 There is no statistical effect due to gradation or compaction method.
9.4 Tensile Strength9.4.1 There is apparently no significant effect due to compaction method but
dense graded (type IV) gradations with Hveem compaction may produce slight higher tensilestrengths.
10.0 Effect of Cure Method
10.1 In an effort to reduce time from compaction to testi~~~ and recognizing thatretained water (lack of cure) has an adverse effect on mixture properties measured in thelaboratory, three methods of cure were studied.
A. 18 hours in compaction mold at room temperature followed by vacuum dessication at 12-15 in.Hg (40.5 - 50.6 kPa) to constant weight. This is the method used to develop data previouslydiscussed and will be referred to as the WTI method.
B. Three day cure in compaction mold at room temperature followed by vacuum dessication at 10-20 mm Hg (1.3 - 2.5 kPa) for 3 days to constant weight. This method is referred to as theChevron method.
C. 24 hours in compaction mold at room temperature followed by 72 hours at 120F (48.9C) with thespecimen placed on a geotextile fabric wick. This method is referred to as the modifiedMonismith or Rapid method.
10.2 Results of this study show no effect of cure method on density but the methoddoes have an effect on resilient modulus, tensile strength, and Hveem stability.
10.3 Resilient Modulus10.3.1 Data for the experiment is shown on Figure 12. There is no significant
difference between the WTI and Rapid methods with a mean of 761,000 psi (5.2 GPa).Both produce a higher modulus than the Chevron method with 388,000 psi (2.7 CPa).
10.4 Tensile Strength10.4.1 Data for the experiment is shown on Figure 13. Trends in tensile strength
follow resilient modulus with no significant difference between the WTI and Rapid methodswith a mean of 108 psi (0.7 MPa) and both produce higher tensile strength than the Chevronmethod with 66 psi (0.5 MPa).
10.5 Hveem Stability10.5.1 Data for the experiment are shown on Figure 14. The Chevron and Rapid
methods produce the same stability (25) and both are significantly lowerthan the WTI method (29).
11.0 Conclusions and Recommendations
11.1 This study, that used kneading compaction, points up some of the same concernsand suggests some of the same conclusions that were made in the first study that used Marshallcompaction. First, is the question of applicability of using conventional hot-mix procedures forthe laboratory evaluation of mixtures using emulsified asphalt. Procedures for hot-mix design(Hveem and Marshall) have been shown to produce laboratory mixtures that fairly accuratelysimulate characteristics of these mixtures after exposure to some traffic. This, and the previousstudy strongly suggest this may not be the case for mixtures using emulsified asphalt binders.
Data from these studies indicate that conventional laboratory compaction methods andprocedures do not produce realistic densities and, hence, show unrealistic low stability whenmeasured in the laboratory. It is recommended that field studies be initiated to determine whatfield density is produced by construction and later traffic compaction and that laboratoryprocedures be modified accordingly. Suggested modifications include study of additional doubleplunger compaction after curing to remove water or preparing specimens for stability testing anddensity-voids analysis by using residue (or base asphalt) rather than the emulsified asphaltbinder.
11.2 The second conclusion that was also made in the first study is that curedemulsified asphalt mixtures show higher resilient moduli at 75F (24C) than mixtures usingconventional asphalt cement binders. The cause of this is not known at this time but it has been
attributed to modification of asphalt properties by the emulsifier. Further study is recommendedto investigate this at higher and lower temperatures, say, 140F (60C) and 0 F (-18C).
11.3 This study showed that curing of laboratory specimens can be accelerated bystoring 72 hours at 120 F (49C) with the specimen placed on a geotextile fabric wick.
Laboratory Specimen Cure Methods
1) 72 hour air cure, out of mold.
2) 24 hour air cure, in mold without weight; 48 hour air cure, out of mold.
3) 24 hour air cure, in mold with 3,000 g load; 48 hour air cure, out of mold.
4) 72 hour in mold, 120F. without weight. 24 hour out of mold, 120F.
5) 72 hour in mold 120F. with 3,000 g load; 24 hour out of mold 120F.
Cure Method Bulk Specific Density Maximum %Air Voids Marshall FlowGravity Theoretical Specific Stability
1 2.15 134 2.46 11.8 3264 172 2.18 136 2.46 10.4 3040 193 2.14 133 2.46 12.1 2980 204 2.26 139 2.46 8.1 3473 135 2.26. 139 2.46 6.3 3411 13
Back to ManualBack to Technical Papers List